- About this Journal
- Abstracting and Indexing
- Aims and Scope
- Article Processing Charges
- Articles in Press
- Author Guidelines
- Bibliographic Information
- Citations to this Journal
- Contact Information
- Editorial Board
- Editorial Workflow
- Free eTOC Alerts
- Publication Ethics
- Reviewers Acknowledgment
- Submit a Manuscript
- Subscription Information
- Table of Contents
Journal of Chemistry
Volume 2013 (2013), Article ID 585920, 7 pages
Photosensitization of Colloidal SnO2 Semiconductor Nanoparticles with Xanthene Dyes
School of Chemistry, Bharathidasan University, Tiruchirappalli, Tamil Nadu 620 024, India
Received 2 May 2013; Revised 18 September 2013; Accepted 19 September 2013
Academic Editor: Veysel T. Yilmaz
Copyright © 2013 N. Nagarajan et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
The photochemical behavior of xanthene dyes (fluorescein, erythrosine, and eosin) with colloidal SnO2 nanoparticles was probed by UV-visible, steady state, and time resolved fluorescence measurements. The prepared SnO2 nanoparticles were characterized by using UV-visible and powder XRD measurements. The xanthene dyes were adsorbed on the surface of colloidal SnO2 nanoparticles through electrostatic interaction. Apparent association constant () was calculated from the relevant fluorescence data. The larger value of apparent association constant indicates a strong association between xanthene dyes and SnO2 nanoparticles. The fluorescence quenching is mainly attributed to electron transfer from the excited state xanthenes to the conduction band of colloidal SnO2. The electron transfer mechanism was explained based on the Rehm-Weller equation as well as the energy level diagram.
The photosensitization of electron transfer across the semiconductor solution interface plays a vital role in light energy conversion in photoelectrochemical cells, wastewater treatment, nanoelectric devices, silver halide photography, and electrophotography. Effort in this area has concentrated on improving the visible light response of wide-band semiconductors such as SnO2, ZnO, and TiO2. Sensitization is achieved by adsorption of dye molecules at the semiconductor surface which, upon excitation, inject an electron into its conduction band [1, 2]. The first successful experiment of this type was described by Putseiko and Terenin  who found that the Dember effect of ZnO powder in visible light was sensitized by xanthene and cyanine dyes.
The investigation and development of the dye-semiconductor systems are essential for various fields of applications. Recently Ferrere et al. and Tian et al. used perylene-SnO2 systems for dye sensitized solar cells [4–6]. The SnO2 is a stable n-type semiconductor with a wide-band gap ( eV) being used for various applications, including solid-state gas sensor, photovoltaic devices, dye-based solar cells, transparent conductive films for display and solar cells, catalysis, and anode materials of secondary lithium ion battery [7–9].
Xanthenes belong to the most widely used organic dyes, serving as luminophores , molecular probes, bioconjugates, stains, and biologically active substances [11, 12]. These dyes are utilized for photosensitization of redox processes [13, 14] in energy transfer and light sensitization studies . They are also used in light-harvesting dendrimers , in biochemistry and medicine as reactants for determination of Zn2+, NO , and H2O2 , in sensor devices for H2S , in studying carbon nanotubes , for creation of water-soluble fluorescent polymers  and new ionic liquids [22–25], and many other fields. Previously we have reported photosensitization of various dyes with semiconductor nanoparticles [26, 27]. The structures of xanthene dyes studied in the present work are shown in Scheme 1.
In the present work, we have studied the interaction between xanthene dyes, namely, fluorescein (FN), eosin (EN), and erythrosine (ERN) with colloidal SnO2 nanoparticles by using steady state and life time measurements. The electron transfer mechanism is proved by Rehm-Weller equation.
2. Experimental Methods
The xanthene dyes were obtained from Aldrich and used without further purification. Dihydrate tin (II) chloride (SnCl2·2H2O) and ethylene glycol (EG) were purchased from Loba, and they were used as such. Double distilled water was used for preparing the solutions throughout. All measurements were performed at ambient temperature.
3.1. Steady-State Measurements
The fluorescence quenching measurements were carried out with JASCO FP-6500 spectrofluorimeter. The slit widths 5 nm and scan rate (500 nm/min) for both excitation and emission were maintained constant for all the measurements. Quartz cells ( cm) with high vacuum Teflon stopcocks were used for measurements. Absorption spectral measurements were recorded using JASCO V630 UV-visible spectrophotometer.
3.2. Time Resolved Fluorescence Measurements
Fluorescence lifetime measurements were carried out in a picosecond time correlated single photon counting (TCSPC) spectrometer. The excitation source was the tunable Ti-sapphire laser (Tsunami, Spectra Physics, USA). The fluorescence decay was analyzed by using the software provided by IBH (DAS-6).
3.3. Powder X-Ray Diffraction Measurements
X-ray diffraction was recorded with a PAN analytical X’ Pert Pro MPD X-ray diffractometer using Cu Kα radiation ( nm) with a Ni filter. The tube current was 30 mA with a tube voltage of 40 kV. The 2θ angular regions between 20 and 80 were explored at a scan rate of 5° min−1.
4. Preparation of Colloidal SnO2 Nanoparticles
Colloidal SnO2 nanoparticles were prepared according to the literature method . In a typical procedure, 0.2 g of SnCl2·2H2O (dissolved in 10 mL of EG) was added to 40 mL of EG that was hosted in a round-bottom flask. After the pH of the solution was kept at 3-4, the solution had been refluxed at 190°C for 2 hours with constant stirring under atmospheric pressure; the clear solution turned into a slight yellow colloid with the reaction time increasing. The resulting SnO2 colloid was used for the further studies.
5. Results and Discussion
5.1. Determination of Particle Size of Colloidal SnO2 Nanoparticles
The relationship between band gap shift () and radius () of the particles is used to determine the particle size by using Brus equation: where is the reduced Planck’s constant, is the radius of the particle, is the effective reduced masses of the and in the semiconductor, is the electron charge, and is the relative permittivity of the semiconductor.
Reduced effective mass of the exciton ()  was used for the calculation. A columbic and polarization term in the equation was neglected. The calculated particle size of the prepared colloidal SnO2 is 1.84 nm.
5.2. XRD Characterization of SnO2 Nanoparticles
To clarify the crystalline structure, an XRD pattern of the SnO2 powder is collected and shown in Figure 1. The diffraction peaks at around 27, 34, 52, and 66° are assigned to SnO2 (110), (101), (211), and (301) (PDF no. 411445), respectively. No diffraction peaks due to metallic Sn or other tin oxides were discerned. The diffraction peaks in the XRD pattern broadened because the particles in the sample are too small. The primary particle size calculated by Scherrer formula is about 1.65 nm.
5.3. Absorption Studies
In an aqueous suspension, the polar surface of metal oxide semiconductor nanoparticles assists adsorption of polar species in solution, and such interactions can lead to absorption spectra changes of these molecules [30, 31]. To find out whether there is any ground state interaction between the sensitizer, that is, xanthene dyes and colloidal SnO2 nanoparticles, ground state absorption measurements of Xanthene in the presence and absence of colloidal SnO2 nanoparticles have been carried out. Figure 2 shows the absorption spectra of FN ( M) in water with different concentrations of SnO2 nanoparticles ( M). Upon increasing the concentration of SnO2 nanoparticles, the absorption decreases gradually . But EN and ERN show red shift with decrease in absorbance (Figures 3 and 4). The presence of an isosbestic point at 531 nm for EN and 543 nm for ERN in these absorptions shows the existence of dye in the adsorbed and unadsorbed state. Such a red shift of 14 nm and 17 nm in the absorption peak indicates a strong interaction of the dye with SnO2 surface. Similar spectral changes have been observed for several organic dyes on metal oxide surfaces .
5.4. Fluorescence Quenching Studies
The excited state interaction between xanthene dyes and SnO2 colloid is observed by spectrofluorimetric measurements. Figure 5 shows the emission spectrum of FN in absence and presence of SnO2 colloid. The fluorescence emission of FN ( M) was quenched upon successive addition of SnO2 colloid (0– M). Other two dyes also show similar type of spectral behavior (spectra are not shown here). The quenching of FN fluorescence by SnO2 colloid can be described by Stern-Volmer: where and are the fluorescence intensities of xanthene dyes in the absence and presence of SnO2 colloid, respectively. is Stern-Volmer constant and  is the concentration of respective quencher. The ratios were calculated and plotted against quencher concentration according to (2).
The Stern-Volmer plot (Figure 6) for EN and ERN is obtained as upward curvature. These types of upward curvature suggest that it may follow static type of mechanism . But, in the case of FN, it gives linear plot. The linear plot mostly results in dynamic quenching. But its value exceeds ( ) the limited values of dynamic quenching ( ), so it also may follow the static quenching.
5.5. Fluorescence Lifetime Measurements
In general, time resolved measurement is the most definitive method for differentiating static and dynamic quenching process. Figure 7 presents a representative plot of the logarithm of the relative fluorescence intensity versus time of EN in absence and presence of SnO2 colloid, from which the lifetimes () of the excited singlet states were obtained by iterative reconvolution of the measured instrument response function. Fluorescence lifetime observed for EN is unchanged with addition of colloidal SnO2. The other two dyes also follow the same trend (spectra are not shown here). This observation shows that quenching follows static mechanism. Static quenching does not decrease the lifetime because only the fluorescent molecules are observed, and the uncomplexed fluorophores have the unquenched lifetime . Static quenching arises due to the formation of complex between fluorophore and the quencher. Hence the association constant () was calculated by the method given below.
The equilibrium between the adsorbed and unadsorbed dye molecules is expressed by using (3); in this equation is the apparent association constant which can be calculated from the fluorescence data by using the reported method : where is the apparent association constant, is the initial fluorescence intensity of dye molecules, is the fluorescence intensity of SnO2 adsorbed dyes, and is the observed fluorescence intensity at its maximum. Figure 8 shows the linear straight line dependence of on the reciprocal concentration of colloidal SnO2. The values are listed in Table 1.
The values decrease in the following order: FN > EN > ERN.
This trend is observed due to the absence of bulkier electronegative group in FN. So the electrostatic interaction between the dye molecule and SnO2 will be more. So it has higher values. But in the case of EN and ERN, it has four bulkier electronegative bromine and iodine atoms. So it has lower values.
5.6. Mechanism of Quenching
The fluorescence quenching of dyes by SnO2 colloid may occur through two possible mechanisms such as energy or electron transfer. There is no overlap between the emission spectra of dyes with the absorption spectrum of SnO2 colloid (Figure 9), and also the band-gap energy of SnO2 ( eV)  is greater than the excited state energy of dyes () shown in Table 2. Thus, energy transfer from excited dyes to SnO2 colloid is not possible. It can therefore be concluded that the fluorescence quenching shown in Figure 5 should not be caused by energy transfer.
The possible way of quenching is through electron transfer from excited state dye molecules to the conduction band of SnO2 colloid as shown in Scheme 2.
The feasibility of electron transfer from dyes to SnO2 can be explained on the basis of energy level diagram based on the excited state oxidation potential of dyes obtained from the oxidation potential of dyes and their singlet state energy according to the equation, , in Table 2, and the conduction band potential of SnO2 lies around 0.0 eV as shown in Scheme 3. From the scheme we observed that the electron transfer process is feasible.
5.7. Calculation of Free Energy Changes () for the Electron Transfer Reactions
To have a better understanding of electron transfer, we have estimated free-energy change () for each dye-SnO2 systems following Rehm-Weller equation : where is the oxidation potential of the donor, is the reduction potential of the acceptor, is the excitation energy of the fluorescent state, and is the columbic term. Since one of the species is neutral and the solvent used is polar in nature, the columbic term in the above expression is neglected . The values thus calculated for the electron transfer processes in the systems studied in water are all negative (Table 2). Hence, the ET processes were thermodynamically feasible .
The effect of colloidal SnO2 nanoparticles on the absorption and fluorescence spectra of dyes such as eosin, erythrosine, and fluorescein has been studied. The result in perturbation of the absorption spectrum shows the surface complex formation through adsorption of dyes on the surface of colloidal SnO2. Static nature of quenching has been confirmed by unaltered fluorescence lifetime from time resolved measurements. Based on the energetic calculations the mechanism of electron transfer from excited state dyes to the conduction band of colloidal SnO2 was suggested.
Conflict of Interests
The authors declare that they have no conflict of interests.
N. Nagarajan thanks DST INSPIRE for the fellowship (IF 10495). R. Renganathan and N. Nagarajan thank DST, India, for their financial support in the form of a Research Grant (Ref. no. SR/S1/PC-12/2011, dt. 20/09/2011). Authors also thank UGC/DST-FIST for UV-VIS and Fluorescence facilities in the School of Chemistry, Bharathidasan University. They are thankful to Professor P. Ramamurthy, NCUFP, University of Madras, Chennai for time resolved measurements.
- J. Moser and M. Gratzel, “Photosensitized electron injection in colloidal semiconductors,” Journal of the American Chemical Society, vol. 106, pp. 6557–6564, 1984.
- C. D. Jaeger, F.-R. F. Fan, and A. J. Bard, “Semiconductor electrodes. 26. Spectral sensitization of semiconductors with phthalocyanine,” Journal of the American Chemical Society, vol. 102, no. 8, pp. 2592–2598, 1980.
- E. K. Putseiko and A. N. Terenin, “Photosensitization of the internal photoeffect in zinc oxide and other semiconductors by adsorbed dyes,” Zhurnal Fizicheskoi Khimii, vol. 23, p. 676, 1949.
- S. Ferrere, A. Zaban, and B. A. Gregg, “Dye sensitization of nanocrystalline tin oxide by perylene derivatives,” Journal of Physical Chemistry B, vol. 101, no. 23, pp. 4490–4493, 1997.
- S. Ferrere and B. A. Gregg, “Large increases in photocurrents and solar conversion efficiencies by UV illumination of dye sensitized solar cells,” Journal of Physical Chemistry B, vol. 105, no. 32, pp. 7602–7605, 2001.
- H. Tian, P.-H. Liu, W. Zhu, E. Gao, D.-J. Wu, and S. Cai, “Synthesis of novel multi-chromophoric soluble perylene derivatives and their photosensitizing properties with wide spectral response for SnO2 nanoporous electrode,” Journal of Materials Chemistry, vol. 10, no. 12, pp. 2708–2715, 2000.
- P. Thangadurai, A. C. Bose, S. Ramasamy, R. Kesavamoorthy, and T. R. Ravindran, “High Pressure effects on electrical resistivity and dielectric properties of nanocrystalline SnO2,” Journal of Physics and Chemistry of Solids, vol. 66, no. 10, pp. 1621–1627, 2005.
- J. A. Toledo-Antonio, R. Gutiérrez-Baez, P. J. Sebastian, and A. Vázquez, “Thermal stability and structural deformation of rutile SnO2 nanoparticles,” Journal of Solid State Chemistry, vol. 174, no. 2, pp. 241–248, 2003.
- A. Y. El-Etre and S. M. Reda, “Characterization of nanocrystalline SnO2 thin film fabricated by electrodeposition method for dye-sensitized solar cell application,” Applied Surface Science, vol. 256, no. 22, pp. 6601–6606, 2010.
- N. Boens, W. Qin, N. Basarić, A. Orte, E. M. Talavera, and J. M. Alvarez-Pez, “Photophysics of the fluorescent pH indicator BCECF,” Journal of Physical Chemistry A, vol. 110, no. 30, pp. 9334–9343, 2006.
- R. P. Haugland, Handbook of Fluorescent Probes and Research Products, Molecular Probes, Eugene, Ore, USA, 9th edition, 2002.
- A. Zumbuehl, D. Jeannerat, S. E. Martin et al., “An amphotericin B-Fluorescein conjugate as a powerful probe for biochemical studies of the membrane,” Angewandte Chemie International Edition, vol. 43, no. 39, pp. 5181–5185, 2004.
- D. C. Neckers and O. M. V. Aguilera, “Photochemistry of the xanthene dyes,” in Advances in Photochemistry, D. H. Volman, G. S. Hammond, and D. C. Neckers, Eds., vol. 18, pp. 313–394, 1993.
- O. Shimizu, J. Watanabe, S. Naito, and Y. Shibata, “Quenching mechanism of rose bengal triplet state involved in photosensitization of oxygen in ethylene glycol,” Journal of Physical Chemistry A, vol. 110, no. 5, pp. 1735–1739, 2006.
- M. H. V. Werts, J. W. Verhoeven, and J. W. Hofstraat, “Efficient visible light sensitisation of water-soluble near-infrared luminescent lanthanide complexes,” Journal of the Chemical Society, no. 3, pp. 433–439, 2000.
- V. Balzani, P. Ceroni, S. Gestermann, M. Gorka, C. Kauffmann, and F. Vögtle, “Fluorescent guests hosted in fluorescent dendrimers,” Tetrahedron, vol. 58, no. 4, pp. 629–637, 2002.
- M. H. Lim, B. A. Wong, W. H. Pitcock Jr., D. Mokshagundam, M.-H. Baik, and S. J. Lippard, “Direct nitric oxide detection in aqueous solution by copper(II) fluorescein complexes,” Journal of the American Chemical Society, vol. 128, no. 44, pp. 14364–14373, 2006.
- H. Maeda, K. Yamamoto, Y. Nomura et al., “A design of fluorescent probes for superoxide based on a nonredox mechanism,” Journal of the American Chemical Society, vol. 127, no. 1, pp. 68–69, 2005.
- C. R. Schröder, B. M. Weidgans, and I. Klimant, “pH fluorosensors for use in marine systems,” Analyst, vol. 130, no. 6, pp. 907–916, 2005.
- N. Nakayama-Ratchford, S. Bangsaruntip, X. Sun, K. Welsher, and H. Dai, “Noncovalent functionalization of carbon nanotubes by fluorescein- polyethylene glycol: supramolecular conjugates with pH-dependent absorbance and fluorescence,” Journal of the American Chemical Society, vol. 129, no. 9, pp. 2448–2449, 2007.
- H. F. Gao, C. C. Wang, W. L. Yang, and S. K. Fu, “Preparation of a water-soluble fluorescent polymer,” Journal of Macromolecular Science A, vol. 41, no. 4, pp. 357–371, 2004.
- N. O. McHedlov-Petrossyan, N. A. Vodolazkaya, Y. A. Gurina, W.-C. Sun, and K. R. Gee, “Medium effects on the prototropic equilibria of fluorescein fluoro derivatives in true and organized solution,” Journal of Physical Chemistry B, vol. 114, no. 13, pp. 4551–4564, 2010.
- J. Pernak, A. Świerczyńska, F. Walkiewicz, E. Krystkowiak, and A. Maciejewski, “Long alkyl chain bis-quaternary ammonium-based ionic liquids as biologically active xanthenes dyes,” Journal of the Brazilian Chemical Society, vol. 20, no. 5, pp. 839–845, 2009.
- M. Ali, V. Kumar, and S. Pandey, “Unusual fluorescein prototropism within aqueous acidic 1-butyl-3-methylimidazolium tetrafluoroborate solution,” Chemical Communications, vol. 46, no. 28, pp. 5112–5114, 2010.
- M. Ali, P. Dutta, and S. Pandey, “Effect of ionic liquid on prototropic and solvatochromic behavior of fluorescein,” Journal of Physical Chemistry B, vol. 114, no. 46, pp. 15042–15051, 2010.
- A. Kathiravan and R. Renganathan, “Effect of anchoring group on the photosensitization of colloidal TiO2 nanoparticles with porphyrins,” Journal of Colloid and Interface Science, vol. 331, no. 2, pp. 401–407, 2009.
- M. A. Jhonsi and R. Renganathan, “Investigations on the photoinduced interaction of water soluble thioglycolic acid (TGA) capped CdTe quantum dots with certain porphyrins,” Journal of Colloid and Interface Science, vol. 344, no. 2, pp. 596–602, 2010.
- L. Jiang, G. Sun, Z. Zhou et al., “Size-controllable synthesis of monodispersed SnO2 nanoparticles and application in electrocatalysts,” Journal of Physical Chemistry B, vol. 109, no. 18, pp. 8774–8778, 2005.
- E. J. H. Lee, C. Ribeiro, T. R. Giraldi, E. Longo, E. R. Leite, and J. A. Varela, “Photoluminescence in quantum-confined SnO2 nanocrystals: evidence of free exciton decay,” Applied Physics Letters, vol. 84, no. 10, pp. 1745–1747, 2004.
- P. V. Kamat, J.-P. Chauvet, and R. W. Fessenden, “Photoelectrochemistry in particulate systems. 4. Photosensitization of a TiO2 semiconductor with a chlorophyll analogue,” Journal of Physical Chemistry, vol. 90, no. 7, pp. 1389–1394, 1986.
- P. V. Kamat, “Photoelectrochemistry in particulate systems. 9. Photosensitized reduction in a colloidal titania system using anthracene-9-carboxylate as the sensitizer,” Journal of Physical Chemistry, vol. 93, no. 2, pp. 859–864, 1989.
- J. Choi, K. Yeo, M. Yoon, S. J. Lee, and K. Kim, “Photoinduced intramolecular charge-transfer state of p-dimethylaminobenzoic acid in CdS and TiO2 colloid solutions,” Journal of Photochemistry and Photobiology A, vol. 132, no. 1-2, pp. 105–114, 2000.
- P. V. Kamat, S. Das, K. G. Thomas, and M. V. George, “Ultrafast photochemical events associated with the photosensitization properties of a squaraine dye,” Chemical Physics Letters, vol. 178, no. 1, pp. 75–79, 1991.
- J. Keizer, “Nonlinear fluorescence quenching and the origin of positive curvature in Stern-Volmer plots,” Journal of the American Chemical Society, vol. 105, no. 6, pp. 1494–1498, 1983.
- J. R. Lakowicz, Principles of Fluorescence Spectroscopy, Plenum Press, NewYork, NY, USA, 1986.
- J.-M. Wu and C.-H. Kuo, “Ultraviolet photodetectors made from SnO2 nanowires,” Thin Solid Films, vol. 517, no. 14, pp. 3870–3873, 2009.
- G. J. Kavarnos and N. J. Turro, “Photosensitization by reversible electron transfer: theories, experimental evidence, and examples,” Chemical Reviews, vol. 86, no. 3, pp. 401–449, 1986.
- S. Parret, F. M. Savary, J. P. Fouassier, and P. Ramamurthy, “Spin-orbit-coupling-induced triplet formation of triphenylpyrylium ion: a flash photolysis study,” Journal of Photochemistry and Photobiology A, vol. 83, no. 3, pp. 205–209, 1994.
- S. Nath, H. Pal, D. K. Palit, A. V. Sapre, and J. P. Mittal, “Steady-state and time-resolved studies on photoinduced interaction of phenothiazine and 10-methylphenothiazine with chloroalkanes,” Journal of Physical Chemistry A, vol. 102, no. 29, pp. 5822–5830, 1998.